Hybrid Silica PVA Nanofibers via Sol Gel Electrospinning silica hybrid nanofibers, the one-step...
Embed Size (px)
Transcript of Hybrid Silica PVA Nanofibers via Sol Gel Electrospinning silica hybrid nanofibers, the one-step...
Hybrid Silica−PVA Nanofibers via Sol−Gel Electrospinning Tahira Pirzada,†,§ Sara A. Arvidson,‡,§ Carl D. Saquing,*,‡,⊥ S. Sakhawat Shah,† and Saad A. Khan*,‡
†Department of Chemistry, Quaid-i-Azam University, Islamabad, 44000, Pakistan ‡Department of Chemical and Biomolecular Engineering, North Carolina State University, Raleigh, North Carolina 27695-7905, United States
*S Supporting Information
ABSTRACT: We report on the synthesis of poly(vinyl alcohol) (PVA)−silica hybrid nanofibers via sol−gel electro- spinning. Silica is synthesized through acid catalysis of a silica precursor (tetraethyl orthosilicate (TEOS) in ethanol−water), and fibers are obtained by electrospinning a mixture of the silica precursor solution and aqueous PVA. A systematic investigation on how the amount of TEOS, the silica−PVA ratio, the aging time of the silica precursor mixture, and the solution rheology influence the fiber morphology is under- taken and reveals a composition window in which defect-free hybrid nanofibers with diameters as small as 150 nm are obtained. When soaked overnight in water, the hybrid fibers remain intact, essentially maintaining their morphology, even though PVA is soluble in water. We believe that mixing of the silica precursor and PVA in solution initiates the participation of the silica precursor in cross-linking of PVA so that its −OH group becomes unavailable for hydrogen bonding with water. FTIR analysis of the hybrids confirms the disappearance of the −OH peak typically shown by PVA, while formation of a bond between PVA and silica is indicated by the Si−O−C peak in the spectra of all the hybrids. The ability to form cross-linked nanofibers of PVA using thermally stable and relatively inert silica could broaden the scope of use of these materials in various technologies.
1. INTRODUCTION Organic−inorganic hybrids are important in a variety of fields as they combine the desirable properties of the inorganic phase (thermal stability, rigidity) with that of the organic phase (flexibility, processability, ductility).1,2 In recent years, poly- mer−silica hybrids with enhanced thermal and mechanical properties2 (because of the silica component), better flexibility (due to the polymer content), and various tailored properties have attracted a lot of attention for a variety of applications including catalysis,3 adsorption,4 pervaporation,5,6 sensors,7 and enzyme encapsulation.8 The scope and utility of these polymer−silica hybrids can be further broadened by trans- forming them to nanofibrous structures that exhibit high surface area to volume ratios.2−4,9,10
Of the various approaches developed to synthesize polymer− silica hybrid nanofibers, the one-step electrospinning process has received a lot of attention due to its simplicity, cost effectiveness, and speed.2,4,11 Electrospinning is a decades-old technique which draws very fine fibers from a viscous liquid (usually a polymer solution or polymer melt) under the force of an electrostatic field.12−16 The resulting fibers have a high surface area to volume ratio that makes them potential candidates for a variety of fields such as membrane technology,17 drug delivery systems,18 enzyme immobiliza- tion,19 electronics,20 and sensors.21 Combining electrospinning with sol−gel processing provides a way to fabricate one-
dimensional nanostructures with tailorable morphologies, size, and composition.22
During the last few decades, the sol−gel method has been widely used to prepare a variety of silica-based materials in forms such as monoliths, powders, tubes, and fibers.23,24 A typical sol−gel process consists of catalyzed hydrolysis and condensation of an initially small molecule (usually an alkoxide) leading to its transformation to an intricate, highly viscous polymeric network and then ultimately resulting in the formation of a ‘gel’ (Scheme I in the Supporting Information). Depending on the composition of the solution and the reaction conditions, the transformation of the sol to the gel state can be modified application requirements.23−25 Since the solution continues to gel over time, there may be only a certain window of time in which the partially gelled solution may be electrospun. Previously, silica nanofibers have been reported from tetraethyl orthosilicate (TEOS) based sol−gels either by pulling the fibers from a sufficiently viscous sol−gel9 or by dry spinning.10 Reports of electrospinning of this type of sol−gel are few, owing to the difficulty of electrospinning a solution that lacks polymer entanglements, and has led to combined sol−gel synthesis/electrospinning with gelators or bind- ers2,4,26−28 to obtain ceramic fibers in the 200−600 nm
Received: January 4, 2012 Revised: March 4, 2012 Published: March 6, 2012
© 2012 American Chemical Society 5834 dx.doi.org/10.1021/la300049j | Langmuir 2012, 28, 5834−5844
range.3,4,26−28 Limited results on electrospun silica nanofibers from a precursor mixture containing TEOS, ethanol, and HCl without any added polymer have also been reported,26 but a systematic study of the variation in properties of the electrospinning solution on the structure of electrospun fibers is not reported. In 2010, Xu et al. provided an account of the synthesis of hybrid silica−yttria and silica−zirconia−yttria fibers through sol−gel electrospinning using a small amount (1− 1.5%) of polyethylene oxide (PEO) as a carrier polymer.27
They examined the changing viscosity of the sol−gel mixture with the passage of time and used a narrow range of solution viscosity (0.3−0.4 Pa s) to produce nonbeaded fibers. However, their objective was to generate dense ceramic nanofibers which were obtained by calcining the polymer content from the nanofibers. Poly(vinyl alcohol) (PVA) is an easily electrospun polymer
that can be used as the organic phase of the polymer−silica hybrid fibers. Its biocompatibility, processability, and hydro- philicity29,30 have led to its industrial use in areas such as membranes,31 adhesives,32 paints, and coatings.30 Water solubility, however, limits PVA use in applications such as ultrafiltration, catalyst support, or biomedical engineering, which require stability in aqueous systems. Research groups are working on chemical or physical cross-linking of PVA to reduce its water solubility using different agents and processes.33−39 Chemical cross-linkers including glutaralde- hyde,35,36,39 hexamethylene diisocyante,33 and maleic acid40
have been used by various research groups to bind the terminal hydroxyl groups of PVA which are mainly responsible for its hydrophilicity;33,35 however, most of these approaches are found to render the material toxic or thermally unstable. Photo- cross-linking34 and freezing−thawing cyclic processing29,37 of PVA offer approaches which produce cross-linked PVA that is nontoxic, but the products are mostly thermally unstable, and the processing requires considerable time and energy expenditures.29,36−39 Therefore, there is a need to develop a PVA composite with reduced water solubility while maintaining the inherent nontoxicity of PVA through a cost-effective approach. Using electrospinning and sol−gel methodologies, we report
a method to prepare silica−PVA composite nanofibers possessing a nonintuitive property of minimal water solubility and provide a description of the molecular interactions to explain the limited solubility of the resulting nanofibers. Since silica is biocompatible, thermally stable, and comparatively inert, incorporation of silica with PVA may produce hybrids with enhanced thermal and chemical stability without relinquishing the biocompatibility of PVA.41,42 Silanol groups on the silica surface (Scheme I in the Supporting Information) are capable of reducing the water solubility of PVA by developing stronger intermolecular interactions, which may result in the improved stability of the hybrid fibers in humid/ aqueous environments. Although there is some work already reported on the synthesis of PVA-templated silica, few research groups have synthesized PVA−silica nanofibers using silicon alkoxide as the precursor.2−4,43,44 In most of the cases, colloidal silica particles were used as the silica source.45,46 Generally, PVA was used to increase the number of entanglements in the silica-containing solution and was later removed to make porous silica fibers;8,47 in cases where PVA was not removed from the hybrid PVA−silica fibers,3,5 the effect of silica on the solubility of PVA was not thoroughly investigated.5,43 Our focus is to spin fibers from solutions containing PVA and a silica
precursor (TEOS) in different ratios as we believe that the proportion of PVA to silanols may affect the ability to form a network; without this network, the solution will not electrospin due to a lack of entanglements. Moreover, by varying the ratio of TEOS:PVA, we can also determine the concentration range of TEOS and PVA in the electrospinning solution that provide high-quality fibers with improved thermal stability, reduced defects, and reduced sensitivity to humid/aqueous conditions. Because of the time dependence of gelation, we studied the effect of aging time of the sol−gel process prior to adding the PVA, which was helpful to conclude whether the silica network or the TEOS is responsible for cross-linking the PVA. Some groups have observed the reduced water solubility of the PVA− silica hybrids,2,6,48 but to our knowledge, no one has studied the morphology and chemistry of water-soaked PVA−silica hybrid fibers in detail or related the changing characteristics (e.g., viscosity, surface tension, conductivity) of the system with the fiber morphology. Fibers